advertisement

International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 12 | Dec 2019 p-ISSN: 2395-0072 www.irjet.net EFFECT ON M30 SCBA CONCRETE IN ACIDIC ENVIRONMENT P. V. RamBabu¹, V. Jahnavi Deepthi², G. V. Ramarao³ ¹Assistant Professor, Department of Civil Engineering, S.R.K.R. Engineering College, Bhimavaram, Andhra Pradesh, India. ²P.G. Student, Department of Civil engineering, S.R.K.R. Engineering college, Bhimavaram, Andhra Pradesh, India. ³Professor, Department of Civil Engineering, Andhra University, Vishakhapatnam, Andhra Pradesh, India. ----------------------------------------------------------------------***--------------------------------------------------------------------ABSTRACT - The usage of blended concrete becoming popular due to the less usage of cement, at the same time the disposal issue of industrial and agricultural wastes can also be reduced. In this experiment we analyze the impact of partial replacement of SCBA in ordinary Portland cement cured in various acidic environments. Bagasse ash has been replaced by 0%, 5%, 10%, 15% and 20% by weight of cement. The concrete specimens were cured for 28, 60 and 90 days in water and in concentrations of 1%, 3 % and 5% sulphuric acid and hydrochloric acid solutions. The tests conducted are compressive strength. The ideal percentage of SCBA replacement is around 10%. The presence of SCBA in concrete developed resistivity towards Acidic attacks. Here, we used the sugar cane bagasse ash as a replacement by 0%, 5%, 10%, 15% and 20% by weight of cement improve quality and reduce the construction cost on materials. The concrete specimens were cured for 28, 60 and 90 days in water and in concentrations of 1%, 3 % and 5% sulphuric acid and hydrochloric acid solutions. The tests conducted are compressive strength. The main objective of this research is to study the durability of sugar cane bagasse ash blended concrete cured in H₂SO4and HCL solution. KEY WORDS: Compressive strength, durability, sugar cane bagasse ash, hydro chloric acid (HCL) and sulphuric acid (H₂SO₄). 2.1. Cement: The most commonly used cement in concrete is ordinary Portland cement of 53 Grade confirming IS 12600- 1989 (2009). 1. INTRODUCTION: 2.2. Fine aggregate: Regionally available river sand, confirming to Zone II as per Indian standards 383-2016. The sand used must be free from clay, silt and other organic impurities. Specific gravity is about 2.6, water absorption is 1% and fineness modulus is around 2.99. In present situation all over the world are seeking on utilization of industrial waste in useful manner, by avoiding disposal problems and landfilling cost [1]. Utilization of various supplementary cementitious materials significantly influences fresh and hardened properties of mortar. Sugarcane bagasse ash is a by-product from sugar industries and can be used as supplementary cementitious material in concrete [2, 3]. When this waste is burned under controlled conditions, it also gives ash having amorphous silica, which has pozzolanic properties. A few studies have been carried out on the ashes obtained directly from the industries to study pozzolanic activity and their suitability as binders, partially replacing cement [4]. Lakshmi Priya [5] investigated the impact of SCBA in concrete by partially replacing SCBA with cement in the ratio of 0%, 5%, 10%, 15%, 20% and 25% by weight for M25 grade of concrete. The experimental study examined the slump of the fresh concrete, compaction factor, compressive strength, split tensile strength, flexural strength, and modulus of elasticity. Vijaya Sehkar Reddy [7] conducted a study where the replacement is done at various percentages like 0%, 5%, 10%, 15% and 20% and its effect on properties of concrete was investigated.. Fresh and hardened properties were exercised with various replacement levels. The study indicated that sugarcane bagasse ash can effectively be used as cement replacement (up to 10%) without substantial change in strength. © 2019, IRJET | Impact Factor value: 7.34 | 2. METHODOLOGY The materials used in this investigation are: 2.3.Coarse aggregate: The crushed aggregate used were 20mm to 12.5mm in size confirming to IS: 10262, IS: 383. Specific gravity is 2.8, water absorption is 0.5% and fineness modulus is 7.26. 2.4. Water: The water that is available in our college campus confirming to the requirement of concreting and curing as per IS: 456-2009. 2.5. Sugar cane bagasse ash: The SCBA which is used in this investigation process was obtained from the KCP Sugar factory, Vuyurru, located in Krishna district, Andhra Pradesh. SCBA contains an approximate 25% of hemi-cellulose, about 25% of lignin and a 50% of cellulose. For each ton of the sugarcane it generates approximately 26% of bagasse at an approximate 50% of moisture content & approximately 0.62% of residual ash. The residue that is left after the combustion gives a chemical composition which is highly dominated by silicon dioxide (SO2). The specific gravity of SCBA was found to be 2.49 ISO 9001:2008 Certified Journal | Page 1140 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 12 | Dec 2019 p-ISSN: 2395-0072 www.irjet.net 4.1. Compressive strength results for cubes cured in water Table-1: Physical properties of sugar cane bagasse ash S. No 1 2 3 4 Property Specific gravity Particle shape Density Specific surface area Test Results 2.49 Spherical 375 Kg/m³ 420 /Kg 3. EXPERIMENTAL PROCEDURE 3.1. Mixing Mixing is done in a pan mixer of 40 liters capacity. The cement materials are thoroughly blended and then to this, the aggregates were added and then completely mixed followed by the slow and gradual addition of water. The mixing has to be done properly until a mixture of uniform colour and consistency are achieved which is ready for casting. Chart-1: CS of SCBA cubes cured in normal water 3.2. Casting of specimen The moulds are cleaned and oil is applied to the mould before concrete is poured into the mould. The moulds are then placed on the level platform. The thoroughly mixed green concrete is filled into the moulds by a vibration method with needle vibrator. Excess concrete was removed and top surface is leveled confirming to IS: 516-1969. Here number of cubes cast are 315, number of cylinders cast are 315 and number of beams cast are 315. The obtained results of SCBA replaced concrete cubes cured in water of all curing periods, the strength variation for 0% to 5% increased up to 2.99% for 28 days, 1.14% for 60 days, 2.3% for 90 days. For 5% to 10% strength increased up to 2.33% for 28 days, 2.81% for 60 days and 2.68% for 90 days. For 10% to 15% strength decreased up to 9.22% for 28 days, 5.47% for 60 days, 7.49% for 90 days and for 15% to 20% strength decreased up to 2.95% for 28 days, 2.4% for 60 days, 2.82% for 90 days. This shows that compressive strength results of SCBA replaced concrete cubes cured in water for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 4.2. Compressive strength results for cubes cured in 1% HCL solution 3.3. Curing the specimen The specimens in the mould are left undisturbed for 24 hours in moulds and then de moulded. De moldings must be done carefully without breaking edges. They must be cured in water, H₂SO4 and HCL solutions for required period confirming to IS: 516-1969. 3.4. Durability The durability tests are conducted on sugarcane bagasse ash concrete against acids such as H₂SO4and HCL. The response of H₂SO4 and HCL attack on sugar cane bagasse ash concrete for various percentages were studied. For conducting this tests concrete specimens like cubes, cylinders and beams with different percentages were casted. The specimens were cured in 1%, 3% and 5% H₂SO4and HCL solutions for different periods of 28, 60 and 90 days. 4. EXPERIMENTAL RESULTS The following graphs shows the mechanical properties of concrete specimens with 0%, 5%, 10%, 15% and 20% weight replacement of cement with SCBA cured in normal water and different percentages of H₂So₄ and HCL solutions for 28, 60 and 90 days. © 2019, IRJET | Impact Factor value: 7.34 | Chart-2: CS of SCBA cubes cured in 1% HCL solution The obtained results of SCBA replaced concrete cubes cured in 1%HCL of all curing periods, the strength variation for 0% to 5% strength increased up to 4.38% for 28 days, 3.23% for 60 days and 8.7% for 90 days. For 5% to 10% strength increased up to 2.7% for 28 days, 2.4%for 60 days and 9.2% for 90 days. For 10% to 15% strength decreased up to 10.4% for 28 days, 14.09% for 60 days and 28.1% for 90 days and for 15% to 20% strength decreased up to 12.9% for 28 days, 12.6% for 60 days and 7.1% for 90 days. This shows that compressive strength results of SCBA replaced concrete cubes cured in 1%HCL for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. ISO 9001:2008 Certified Journal | Page 1141 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 12 | Dec 2019 p-ISSN: 2395-0072 www.irjet.net 4.3. Compressive strength results for cubes cured in 3% HCL solution 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 4.5. Compressive strength results for cubes cured in 1% H₂So₄ solution Chart-3: CS of SCBA cubes cured in 3% HCL solution The obtained results of SCBA replaced concrete cubes cured in 3%HCL of all curing periods, the strength variation for 0% to 5% strength increased up to 7.04% for 28 days, 5.8% for 60 days and 11.9% for 90 days. For 5% to 10% strength increased up to 4.99% for 28 days, 4.93% for 60 days and 2.47% 90 days, for 10% to 15% strength decreased up to 20.9% for 28 days, 22.77% for 60 days and 26.17% for 90 days and for 15% to 20% strength decreased up to 16.7% for 28 days, 21.47% for 60 days and 1.67% for 90 days. This shows that compressive strength results of SCBA replaced concrete cubes cured in 3% HCL for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 4.4. Compressive strength results for cubes cured in 5% HCL solution Chart-5: CS of SCBA cubes cured in 1% H₂So₄ solution The obtained results of SCBA replaced concrete cubes cured in 1% H₂So4 of all curing periods, the strength variation for 0% to 5% strength increased up to 4.13% for 28 days, 6.47% foe 60 days, 19.94% for 90 days. For 5% to 10% strength increased up to 2.64% for 28 days, 5.92% for 60 days and 6% for 90 days. For 10% to 15% strength decreased up to 13.72% for 28 days, 12.23% for 60 days, 24.69% for 90 days and for 15% to 20% strength decreased up to 9.95% for 28 days, 13.17% for 60 days, 7.97% for 90 days. This shows that compressive strength results of SCBA replaced concrete cubes cured in 1% H₂So4 for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 4.6. Compressive strength results for cubes cured in 3% H₂So₄ solution Chart-4: CS of SCBA cubes cured in 5% HCL solution The obtained results of SCBA replaced concrete cubes cured in 5%HCL of all curing periods, the strength variation for 0% to 5% strength increased up to 4.12% for 28 days, 8.5% for 60 days and 9.3% for 90 days. For 5% to 10% strength increased up to 4.7% for 28 days, 4.4% for 60 days and 4.6% for 90 days. For 10% to 15% strength decreased up to 22.3% for 28 days, 28.07% for 60 days and 29.2% for 90 days and for 15% to 20% strength decreased up to 24.6% for 28 days, 18.5% for 60 days and 20.88% for 90 days. This shows that compressive strength results of SCBA replaced concrete cubes cured in 5% HCL for all curing periods increase up to © 2019, IRJET | Impact Factor value: 7.34 | Chart-6: CS of SCBA cubes cured in 3% H₂So₄ solution The obtained results of SCBA replaced concrete cubes cured in 3% H₂So4 of all curing periods, the strength variation for 0% to 5% strength increased up to 4.85% for 28 days, 7.04% for 60 days, 19.12% for 90 days, for 5% to 10% strength increased up to 6.73% for 28 days, 3.56% for 60 days and 4.04% for 90 days, for 10% to 15% strength decreased up to 21% for 28 days, 22.89% for 60 days, 26.67% for 90 days and for 15% to 20% strength decreased up to 8.28% for 28 days, 13.51% for 60 days, 12.84 % for 90 days. This shows that compressive strength of SCBA replaced concrete cubes ISO 9001:2008 Certified Journal | Page 1142 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 12 | Dec 2019 p-ISSN: 2395-0072 www.irjet.net cured in 3% H₂So4 for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 6. REFERENCES 1. Akash G S, Madhukar K, Chetan T, Aishwarya T, Dinesh S Magnur, Dr. Sivakumar B, “Experimental Study On Partial Replacement Of Sand With Sugarcane Bagasse Ash In Concrete”, International Research Journal of Engineering and Technology (IRJET), Volume: 05 Issue: 5, May-2018. 4.7. Compressive strength results for cubes cured in 5% H₂So₄ solution 2. Alireza Joshaghani, Ali Akbar Ramezanianpour, Hossein Rostami, “Effect of incorporating Sugarcane Bagasse Ash (SCBA) in mortar to examine durability of sulphate attack”, ResearchGate, Conference Paper· June 2016 3. BangarSayali S, PhalkeShubhangi N, Gawade Anjali Y, Tambe Rutuja S and Rahane A. B, “A Review Paper On Replacement Of Cement With Bagasse Ash”, International Journal Of Engineering Sciences and Management, March 2017 Chart-7: CS of SCBA cubes cured in 5% H₂So₄ solution The obtained results of SCBA replaced concrete cubes cured in 5% H₂So4 of all curing periods, the strength variation for 0% to 5% strength increased up to 9.2% for 28 days, 11.73% for 60 days, 9% for 90 days. For 5% to 10% strength increased up to 5.09% for 28 days, 7.76% for 60 days and 13.57% for 90 days. For 10% to 15% strength decreased up to 27.75% for 28 days, 31.35% for 60 days, 21.16% for 90 days and for 15% to 20% strength decreased up to 13.07% for 28 days, 4.67% for 60 days, 18.26% for 90 days. This shows that compressive strength of SCBA replaced concrete cubes cured in 5% H₂So4 for all curing periods increase up to 10% replacement and a decrease in compressive strength is observed at 15% and 20% replacements. 5. CONCLUSIONS It was observed that due to the presence of high amount of silica in SCBA, the concrete blended with 10% SCBA by weight of cement has more strength when compared to ordinary concrete in all curing conditions. There is a decrease in strength and increase in slump after addition of SCBA beyond 10% SCBA replacement by weight of cement. The strength increased in SCBA concrete specimens cured in 1% hydrochloric acid and sulphuric acid solution when compared with specimens cured in normal concrete at 90 days. SCBA replaced concrete specimens produced maximum compressive strength when cured in both sulphuric acid and Hydrochloric acid when compared with normal concrete. The presence of SCBA in concrete developed resistivity towards Acidic attack. © 2019, IRJET | Impact Factor value: 7.34 | 4. Jayminkumar A. Patel, D. B. Raijiwala, “Experimental Study on Use of Sugar Cane Bagasse Ash in Concrete by Partially Replacement with Cement”, International Journal of Innovative Research in Science, Engineering and Technology, Vol. 4, Issue 4, April 2015. 5. K. Lakshmi Priya, R. Ragupathy, “Effect of Sugarcane Bagasse Ash on Strength Properties of Concrete”, International Journal of Research in Engineering and Technology (IJRET), 2016, Vol. 05, No. 04, pp. 159-164. 6. Khansaheb A. P, “Experimental Investigation on Properties of Concrete Using Human Hair & Sugarcane Bagasse Ash”, International Journal of Innovative and Emerging Research in Engineering Volume 2, Issue 5, 2015 7. M. Vijaya Sekhar Reddy, K. Ashalatha, M. Madhuri, P. Sumalatha, “Utilization of Sugarcane Bagasse Ash (SCBA) In Concrete By partial Replacement Of Cement”, International Organization of Scientific Research Journal of Mechanical and Civil Engineering (IOSR-JMCE), 2015, Vol. 12, No. 06, pp. 12-16. 8. M. S. Chennakesava Rao, N. V. N. Prabath, “Green Concrete using Agro Industrial Waste (Sugarcane Bagasse ASH)”, International Journal of Soft Computing and Engineering (IJSCE)ISSN: 2231-2307, Volume-5 Issue-1, March 2015 9. P V Rambabu, G. Aditya, G V Ramarao, “Effect of Acidic Environment (HCL) on Concrete With Sugarcane Bagasse Ash As Pozzolana”, International Journal of Engineering Research and Applications (ijera)ISSN: 2248-9622, Vol. 5, Issue 11, (Part - 4) November 2015, pp.59-64 10. T. S. Abdulkadir, D. O. Oyejobi, A. A. Lawal, “Evaluation of sugercane bagasse ash as a replacement for cement in concrete works”, ACTA TEHNICA CORVINIENSIS – Bulletin of Engineering, Tome VII, Fascicule 3, September 2014. ISO 9001:2008 Certified Journal | Page 1143 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 12 | Dec 2019 p-ISSN: 2395-0072 www.irjet.net 11. T. Subramani, M. Prabhakaran, “Experimental Study On Bagasse Ash In Concrete”, International Journal of Application or Innovation in Engineering & Management (IJAIEM), Volume 4, Issue 5, May 2015 12. U.R.Kawade1, Mr.V.R.Rathi2, Miss Vaishali D. Girge, “Effect of use of Bagasse Ash on Strength of Concrete”, International Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013 © 2019, IRJET | Impact Factor value: 7.34 | ISO 9001:2008 Certified Journal | Page 1144